Click here to load reader
Click here to load reader
Jul 29, 2020
Journal of Saudi Chemical Society (2014) xxx, xxx–xxx
King Saud University
Journal of Saudi Chemical Society
On different photodecomposition behaviors of rhodamine B on laponite and montmorillonite clay under visible light irradiation
Peng Wang *, Mingming Cheng, Zhonghai Zhang
Water Desalination and Reuse Center, Division of Biological and Environmental Science & Engineering, King Abdullah University of Science and Technology, Thuwal 23955-6900, Saudi Arabia
Received 17 September 2013; revised 13 November 2013; accepted 18 November 2013
P m j.
Corresponding author. Tel.:
mail address: [email protected]
er review under responsibilit
lease cite this article in pr ontmorillonite clay unde
19-6103 ª 2013 King Saud U tp://dx.doi.org/10.1016/j.jscs.
y of King
ess as: P r visibl
Abstract In this study, laponite and montmorillonite clays were found to be able to decompose
rhodamine B upon visible light irradiation (k > 420 nm). Very interestingly, it was found that rho- damine B on laponite underwent a stepwise N-deethylation and its decomposition was terminated
once rhodamine 110, as a decomposition product, was formed, whereas the same phenomenon was
not observed for rhodamine B on montmorillonite, whose decomposition involved chromophore
destruction. Mechanistic study revealed that the different photodecomposition behaviors of rhoda-
mine B on laponite and montmorillonite were attributed to the oxidation by different reactive oxy-
gen species, with laponite involving HO�2=O �� 2 while montmorillonite involving
�OH. It was also
found that the degradation pathway of rhodamine B on laponite switched from N-deethylation
to chromophore destruction when solution pH was changed from 7.0 to 3.0, which was attributed
to a much higher fraction of HO�2 relative to O �� 2 under pH 3.0 than under pH 7.0. Based on the
results, a mechanism of rhodamine dye decomposition on clay under visible light was proposed,
involving the clay as an electron acceptor, electron relay between the adsorbed dye molecules
and oxygen molecules, and subsequent reactions between the generated dye radical cations and dif-
ferent reactive oxygen species. The results of this study shed light on how to best utilize visible light
for organic pollutant degradation on clays within engineered treatment systems as well as on many
of naturally occurring pollutant degradation processes in soils and air involving clay. ª 2013 King Saud University. Production and hosting by Elsevier B.V. All rights reserved.
a (P. Wang).
g by Elsevier
. Wang et al., On different ph e light irradiation, Journal o
. Production and hosting by Elsev
Clay has long been employed as catalysts, adsorbents, and host materials in many of industrial, agricultural, and environmen-
tal decontamination processes and many of the clay applica- tions are based on clay-organic interactions [16,29,33,36]. Generally, organic molecules interact with clay surfaces via the following mechanisms: (1) electrostatic interaction of ionic
otodecomposition behaviors of rhodamine B on laponite and f Saudi Chemical Society (2014), http://dx.doi.org/10.1016/
ier B.V. All rights reserved.
mailto:[email protected] http://dx.doi.org/10.1016/j.jscs.2013.11.006 http://dx.doi.org/10.1016/j.jscs.2013.11.006 http://www.sciencedirect.com/science/journal/13196103 http://dx.doi.org/10.1016/j.jscs.2013.11.006 http://dx.doi.org/10.1016/j.jscs.2013.11.006 http://dx.doi.org/10.1016/j.jscs.2013.11.006
2 P. Wang et al.
organic species with charged clay surfaces; (2) complexation of organic species with clay surfaces; for example, the p electrons of the phenyl in dioxins react with Lewis acid sites on laponite
surfaces to form p electron complexes ; (3) coordination of nonionic species, such as alcohols, ketones, pyridines, with exchangeable metallic ions on clay surfaces [33,29].
Dye molecules, especially rhodamine dyes, are among the most commonly utilized probe molecules in studying clay-or- ganic interactions in aqueous solutions (Martı́nez et al.,
2005; Martı́nez et al., 2006; ; 2006). Two-dimensional clay surface provides a rigid microenvironment for the dye mole- cules to adsorb. Adsorption is usually a prerequisite for a pho- tochemical reaction of the organic dyes to occur with the clay
as the adsorbed dye molecules self-assemble on the clay sur- faces to form molecular aggregates, leading to a photon- responsive hybrid material [24,4]; . Photoinduced electron
transfer, involving the adsorbed molecules and the clay, is one of the most known initiation steps for the photochemical reaction of the adsorbed molecules to proceed. For example,
UV irradiation induced guest-to-host electron transfer and subsequent catalytic oxidation of pyrene [19,18,34], thianth- rene , dioxin , and biphenyl  have been reported
on laponite. In most cases, clays act as electron acceptors during the
electron transfer processes. It is known that the external sur- face of clay is built up of outer surface and lateral surface
(i.e., edges). For example, the outer surface of laponite in- volves siloxane bonds while its lateral surface includes broken and terminated Si–O, Mg–O and/or Li–O bonds. These ex-
posed structural metal cations at the edges are electron-defi- cient or Lewis acid sites, which are generally recognized as electron acceptors [19,25,5,31]. Following an electron transfer
from the adsorbed organic molecules to the acceptor sites on the clays, organic radical cations are thus generated. It is be- lieved that the ionic and high polarity nature of the clay sur-
faces stabilizes the formation and increases the yield of these radicals , making the clays ideal materials for photochem- ical studies.
In some other cases, clays may serve as electron donors dur-
ing an electron transfer. For example oxygen lone pair in Si– O–Al of smectite is able to donate one electron to the excited methyl viologen (MV2+) to form MV�+ . Similar process
has been reported to lead to a photodegradation of decabro- modiphenyl ether .
UV-induced organic molecule decomposition on clay has
been widely examined so far, but there has been little investiga- tion on visible light induced organic decomposition [20,1,26], especially on the decomposition behaviors of organic dyes on clay surfaces. Since dye molecules adsorbed on clay can be
potentially excited by visible light irradiation , an electron transfer between the adsorbed dye molecules and the electron acceptor sites on the clay surfaces might lead to a charge sep-
aration and subsequent formation of dye radical cations. It is thus expected that the formed dye radical cations can undergo hydrolysis or reactions with active oxygen species (e.g., HO�2 ,
O��2 , �OH) present within the system, which may lead to a
decomposition of the dye. As UV accounts for only less than 5% while visible irradiation makes up 50% of the total solar
energy , investigation of visible irradiation assisted photo- decomposition of dyes on clay is much needed as it will shed light on how to best utilize visible light for organic pollutant
Please cite this article in press as: P. Wang et al., On different ph montmorillonite clay under visible light irradiation, Journal o j.jscs.2013.11.006
degradation on clays within engineered treatment systems as well as on many of naturally occurring pollutant degradation processes in soils [14,15] and air  involving clay.
The objectives of this study are (1) to explore the visible light photodecomposition chemistry of rhodamine B on two clays, laponite and montmorillonite, which represent synthetic
clays with a high purity and natural ones with such impurities as iron, respectively; (2) to propose and discuss the mechanism of rhodamine dye photodecomposition on clay under visible
2. Experimental section
2.1. Materials and reagents
Montmorillonite, with a cation exchange capacity (CEC) of 100 meq/100 g, was purchased from Sigma–Aldrich (Montmo- rillonite K10) and treated as previously reported to remove metal impurities . The as-obtained Na-montmorillonite
(hereafter MMT) had a structural Fe content of 2.05% as determined by Inductively Coupled Plasma-Atomic Emission Spectroscopy (ICP-AES). Laponite, with a CEC of 55 meq/
100 g, was supplied by Fernz Specialty Chemicals, Australia. Na-saponite (JCSS-3501, Kunimine Industry Co. Ltd.) was purchased from Clay Science Society of Japan. CEC of the
saponite is 100 meq/100 g. Both laponite and saponite are syn- thetic materials (diffuse reflectance UV–vis spectra are pre- sented in Figure S1). The main advantage of using these
synthetic clays is that they are available in a high degree of purity and contain essentially no other active metal atoms such as Fe3+ and Cu2+. Barnstead UltraPure water (18.3 MX) was used throughout the study. Horseradish peroxidase (POD)
used for H2O2 measurement was purchased fro